arxiv: v1 [condmat.strel] 6 Feb 2008

 Ezra Copeland
 5 months ago
 Views:
Transcription
1 Large Magnetoresistance in a Manganite SpinTunnelJunction Using LaMnO 3 as Insulating Barrier S. Yunoki, and E. Dagotto Department of Physics and Astronomy, The University of Tennessee, Knoxville, Tennessee 37996, USA, and Materials Science and Technology Division, Oak Ridge National Laboratory, Oak Ridge, Tennessee 32831, USA. arxiv: v1 [condmat.strel] 6 Feb 2008 S. Costamagna and J. A. Riera Instituto de Física Rosario, Consejo Nacional de Investigaciones Científicas y Técnicas, Universidad Nacional de Rosario, Rosario, Argentina (Dated: February 8, 2008) A spintunneljunction based on manganites, with La 1 xsr xmno 3 (LSMO) as ferromagnetic metallic electrodes and the undoped parent compound LaMnO 3 (LMO) as insulating barrier, is here theoretically discussed using double exchange model Hamiltonians and numerical techniques. For an even number of LMO layers, the ground state is shown to have antiparallel LSMO magnetic moments. This highly resistive, but fragile, state is easily destabilized by small magnetic fields, which orient the LSMO moments in the direction of the field. The magnetoresistance associated with this transition is very large, according to Monte Carlo and Density Matrix Renormalization Group studies. The influence of temperature, the case of an odd number of LMO layers, and the differences between LMO and SrTiO 3 as barriers are also addressed. General trends are discussed. PACS numbers: f, w, c, b I. INTRODUCTION The study of strongly correlated electronic systems (SCES) continues attracting the attention of the Condensed Matter community. These materials present complex phase diagrams that illustrates the competition which exists among phases with very different physical properties, such as dwave superconductivity, antiferroand ferromagnetic order, charge and orbitalorder, multiferroic behavior, and several others. Moreover, this complexity and phase competition lead to selforganized nanoscale inhomogeneities which are believed to generate giant responses, as in the famous colossal magnetoresistance (CMR) effect of the Mnoxides known as manganites. 1 Recently, a new procedure to study oxide SCES has been proposed. It involves the artificial creation of oxide multilayers with atomicscale accuracy at the interface, via the use of techniques such as pulsedlaser deposition. 2 Potentially, these structures can have properties very different from those of the building blocks. One of the reasons for this expectation is that a transfer of charge could occur between the constituents leading, for example, to the stabilization of a metal at the interface between two insulators. 2 The creation of novel twodimensional states, as well as the possible applications of oxide multilayers in the growing field of oxide electronics, has given considerable momentum to these investigations. A. SpinTunnelJunctions The development of the above mentioned accurate experimental techniques for the construction of oxide multilayers with atomic precision can have implications in the study of spintunneljunctions, 3,4 introducing a better control of their properties. These structures consist of two ferromagnetic (FM) metallic electrodes, separated by a thin insulating barrier. The resistance of this device depends on the relative orientation of the electrodes magnetizations. The tunneling magnetoresistance (TMR) is usually defined via the difference in resistances between the antiparallel and parallel arrangements of the electrodes magnetic moments. Halfmetals, such as La 1 x Sr x MnO 3 (LSMO), with an intrinsic nearly full magnetization, are ideal for these devices. 5 In the context of magnetic tunnel junctions, very interesting results were reported by Bowen et al. 6 using a LSMO/STO/LSMO trilayer. The Sr concentration was 1/3 for La 1 x Sr x MnO 3 (LSMO), and STO represents the insulator SrTiO 3. A huge TMR ratio of more than 1800% was observed at very low temperatures 4 K, showing the advantages of using halfmetallic LSMO as a ferromagnetic electrode in the junctions. However, in the same investigations it was reported that the large TMR survived only up to 270 K, lower than the Curie temperature of LSMO(x=1/3), which is 370 K. It was argued that the deterioration of the ferromagnetism near the LSMO/STO interface ( dead layer ) could be causing this TMR reduction. Later, Yamada et al. 7 addressed this problem by comparing the STO/LSMO interface with others, such as LAO/LSMO or STO/LMO/LSMO, where LAO stands for LaAlO 3 and LMO for LaMnO 3. Those authors found that the magnetic behavior of LAO/LSMO and STO/LMO/LSMO are much better than STO/LSMO in the sense that no deadlayer was found, opening a new path toward LSMObased TMR junctions operating at room temperature.
2 2 B. Proposed Main Idea (a) In this paper, an alternative setup is proposed for a manganite trilayer system which is expected to have a very large magnetoresistance (MR) at low temperatures, at least according to modeling calculations reported below. The proposed geometry, and main idea behind its performance, is presented in Fig. 1. The new system is made out entirely of manganite materials, with different hole doping concentrations. 8 Using all manganites may help in the interfacial contact between the components due to their similar lattice spacings. More specifically, in Fig. 1 (a) a trilayer system is represented. It contains two holedoped Mnoxides, such as LSMO, and a central region made out of the undoped parent compound LMO. It is well known that LSMO is ferromagnetic and halfmetallic for sufficiently large hole doping, while LMO is an Atype antiferromagnetic (AF) insulator. 1 The arrows in Fig. 1 (a) represent schematically the expected spin orientations in a onedimensional arrangement, for simplicity. The most interesting detail of Fig. 1 (a) is the relative orientation of the spins between the metallic leads. For an even number of layers in the central LMO region, the ferromagnetic moments of the leads are antiparallel. This is expected to cause a very large resistance at low temperatures, since the carriers moving from one lead to the other not only must tunnel through the central insulating barrier, but in addition the spin species which can travel in one lead is blocked by the other. However, the antiparallel configuration, which is mediated by the central region, is not strongly pinned in this arrangement: it is only a weak antiferromagnetic effective interaction which produces the ground state with antiparallel leads moments. Thus, relatively small magnetic fields can render the ferromagnetic moments parallel, substantially reducing the resistance. All these intuitive ideas will be substantiated via model calculations, described below. For an odd number of layers in the central LMO region, the expected spin arrangement is shown in Fig. 1 (b). In this case the magnetic moments of the leads will be parallel to one another, and the resistance will not be as large as for the configuration shown in Fig. 1 (a). However, the LMO region still provided a tunneling barrier, and the performance of this case will be shown below to be quite acceptable, at least within modeling calculations. Finally, Fig. 1(c) contains a crude representation of a more standard trilayer device. 6 While the leads are still representing LSMO, the central region is now a band insulator, as it occurs in the much employed case of STO. The main focus of our effort will be the cases shown in Fig. 1 (a) and (b), but some results for the setup shown in Fig. 1 (c) will also be discussed for completeness, and to clarify qualitative trends. (b) (c) FM FM FM AFM AFM V m FIG. 1: (Color online) Schematic representation of a onedimensional (1D) double exchange (DE) model for a LSMO/LMO/LSMO trilayer with even (a) and odd (b) numbers of LMO sites. Here, LMO and LSMO represent regions where the positive background charge densities correspond to an antiferromagnetic (AFM) insulator and ferromagnetic (FM) metal, respectively, when in bulk form. Circles stand for lattice sites where electrons can move, and arrows indicate localized spins. The trilayer with even (odd) number of LMO sites gives rise to antiparallel (parallel) alignment of the magnetic moments in the left and right ends of LSMO. (c) Schematic representation of a 1D model for a LSMO/STO/LSMO trilayer. Here, LSMO is described by the DE model as before, while STO is modeled by a tightbanding model with no localized spins. V m introduced in the central STO region is a band offset sitepotential mimicking the work function difference between LSMO and STO. More details can be found in the text. C. Main approximations Before proceeding to the presentation of the results, some of the theoretical approximations used must be clearly expressed for the benefit of the reader. With this paper, our main intention is to motivate experimental groups to consider the materials and setups proposed in our study, involving a magnetically active manganite barrier, as opposed to a magneticallyinert bandinsulator, as the widely used STO. However, it must be clearly stated that our calculations are qualitative at best and should be considered only as a guidance to understand the intuitive picture presented here. A variety of effects are not taken into account in this investigation (and actually these effects cannot be taken into account accurately within the current status of numerical simulations and Hamiltonian modeling). (1) For instance, the lattice and orbital reconstructions are not incorporated, but only the electronic reconstruction is considered. In other words, the atomic positions are con FM FM FM
3 3 sidered to be rigid here. It would be the task of sophisticated abinitio simulations to consider how the lattice relaxes at the interface between LMO and LSMO, and such future calculations are certainly strongly encouraged. (2) A second subject which is not addressed in this work is the issue of the infamous dead layer at the barrier/electrode interface, already briefly described in Sec. I A. Dead layers affect the performance of several trilayer devices. We have attempted to mimic this dead layer altering by hand the chemical potential in the vicinity of the interface, but the results were not sufficiently satisfactory to be described in this paper. Thus, this problem is left for future efforts. (3) Another topic which is only briefly discussed is the influence of anisotropies: in most of the simulations below there is no easy axis introduced for the magnetization orientation. While for manganites in bulk form this is a reasonable assumption, in thin films it is known that inplane magnetic anisotropies are induced by epitaxial strain. 9 These anisotropies are the reason behind the abrupt changes in resistances observed when varying magnetic fields in magnetic tunnel junctions (see, for instance, Fig. 2 in Ref. 6). While in our numerical studies reported below the simulations are carried out mainly with isotropic Heisenberg spins, a more proper analysis would have needed anisotropic terms, rendering these spins Ising like. (4) A related topic involves the experimentally observed differences between the upper and lower electrodes in a trilayer junction, since the area of the bottom electrode is typically much wider than that of the upper one. 10 This stabilizes antiparallel orientations of the electrodes magnetic moments at some magnetic fields. In our simulations, both electrodes are perfectly equivalent. However, for the reasons already mentioned in the previous subsection, we do stabilize a similar antiparallel magnetic moment arrangement via the use of LMO as barrier, with an even number of sites and in zero external magnetic field. (5) Finally, a practical assumption in our investigations is the focus on a onedimensional (1D) spin arrangement, described by the realistic doubleexchange model for manganites (albeit restricted to just one orbital). The restriction to a 1D configuration is needed for the numerical studies to be accurate; higher dimensional arrangements would have increased so much the CPU time that a careful analysis would have been impossible. Note that contrary to manganite bulk studies, 1 where the analysis of small twodimensional clusters is possible, here we will be carrying out an iterative loop to solve Poisson s equation which regulates the charge transfer between materials (see Sec.II). At each step of the iterative process, an entire Monte Carlo (MC) process or Density Matrix Renormalization Group (DMRG) sweep is carried out (see details below), thus increasing substantially the computer requirements. Then, the restriction to a 1D geometry is caused by the CPU resources available. However, in the description of results below, we have focus on qualitative aspects which are expected to be robust, and we strongly believe that they will survive the increase in dimensionality. For example, the large magnetoresistance at low temperatures of the LSMO/LMO/LSMO setup, with an even number of layers for LMO, is believed to occur in any dimension of interest. D. Organization The organization of the paper is the following. In Sec. II, the model Hamiltonians and numerical methods are described. The focus is on Monte Carlo and DMRG techniques. The main results are presented in Sec. III, which correspond to the arrangements schematically described in Fig. 1 (a) and (b), showing that the magnetoresistance is large in these setups. Both classical and quantum localized t 2g spins are used. In Sec. IV, the influence of temperature is analyzed. As observed in some experiments, 6 it is found that the large MR effect quickly deteriorates with increasing temperature. The influence of anisotropies is also studied as a possible cure to this problem. In Sec. V, for completeness, results of the modeling of a trilayer involving a band insulator (such as STO) as the barrier, instead of LMO, are reported. Conclusions are given in Sec. VI. II. MODEL AND METHODS A. Model Hamiltonian and MC methods To crudely model LSMO/LMO/LSMO trilayers (Fig. 1), the oneorbital double exchange (DE) model on a 1D lattice will be used: H = t ( ) c i,σ c j,σ + H.c. + φ(i)n i i,j σ i J H s i S i h ext M i, (1) i i where c i,σ is the creation operator of an electron at site i with spin σ(=, ). The first summation of i, j runs over nearest neighbor pairs of sites i and j. The number operator is n i = σ c i,σ c i,σ, φ(i) is the electrostatic potential (discussed below), and the spin operator of the electron is s i = α,β c i,α ( σ) αβ c i,β (here σ = (σ x, σ y, σ z ): Pauli matrices). S i is the classical spin, widely used to represent the localized t 2g spins, with S i =1. J H is the Hund s rule coupling, h ext is an external magnetic field, and M i = 1 2 (s i + 3S i ) is the total magnetic moment at site i. Hereafter, t is set to be 1 as an energy unit. The number of sites in the left, central, and right regions of the system is denoted by L (L), L (C), L (R), respectively. To study the electronic properties of heterostructured systems, it is crucial to include the cation ions in the model (to consider the charge neutrality condition) and
4 4 take into account longrange Coulomb interactions between electrons and cation ions. In this study, the longrange Coulomb interactions are considered within the Hartree approximation through Poisson s equation: 11 2 φ(i) = α [ n i n + (i)], (2) where n + (i) is the positive background charge mimicking the cation ions. Here in this paper, n + (i)=n (Γ) is set to be uniform within each layer [Γ=L (left region), C (central region), and R (right region)], with a value determined by the charge neutrality condition. The parameter α=e 2 /εa (e: electronic charge, ε: dielectric constant, a: lattice constant) is the strength of the Coulomb interactions, considered as a free parameter in the model. To solve Eq. (2), the symmetric discretization of Poisson s equation is used, which in 1D becomes 2 φ(i)=φ(i + 1) 2φ(i) + φ(i 1), with boundary conditions φ(i)=0 for sites outside of the system. In the following sections, results for zero temperature (T) as well as finite temperatures are reported. For the finite temperature calculations, the standard grandcanonical Monte Carlo simulation is used, 12 with the chemical potential µ adjusted such that the total number of electrons are equal to the total background positive charge i n +(i). For the zero temperature calculations, a full optimization of {S i } using the BroydenFletcher GoldfarbShanno method 13 is performed for a fixed number N of electrons, i.e., N = i n +(i) (canonical ensemble). We have found that the Monte Carlo simulations at very low temperatures produce almost identical results as those calculated using the zero temperature canonical method, although at a considerably larger cost in CPU time. Thus, at T=0 it is advantageous to use the optimization method. Note that due to the need to solve Poisson s equation iteratively, a Monte Carlo simulation or optimization procedure has to be carried out at each step, increasing substantially the computer time as compared with more standard simulations of bulk systems. The calculation of the conductances is carried out using the Landauer formalism, 14 as extensively explained in previous reports. 1,15 In the real LSMO/STO/LSMO trilayer systems, which will also be briefly modeled in this manuscript, it is important to notice that there exists band offsets (due to workfunction differences) between LSMO and STO, which are typically of the order of a few evs, 16 although its precise value is difficult to find experimentally. 17 In this paper, this band offset is treated as a parameter described simply by the addition of a site potential term V m i C n i to the Hamiltonian [Fig. 1 (c)]. Moreover, a simple tightbinding model without J H in Eq. (1) is used to model the STO barrier. Omitting Hubbardtype interactions might be justified by the fact that the number of electrons in the central region (STO) is very small, as shown later. And for LSMO and LMO, neglecting the Hubbard term is justified by the large value of the Hund s coupling which by itself prevents double occupancy, as widely discussed before. 1 B. Quantum localized spins and DMRG Results using quantum spin 1/2 for the localized spins S i in Eq. (1) are also presented in this paper, and they are compared with results of the classical spin simulations. In real manganites t 2g spins are 3/2. However, using spin 1/2 much simplifies the computational task due to the reduction in the size of the Hilbert space. 12 To study the ground state properties of Eq. (1) with S i = 1/2, e.g., the charge density distribution, the standard DMRG algorithm, 18 embedded in a selfconsistent iterative procedure to solve Poisson s equation for the longrange Coulomb potential, is used. More specifically, starting from an initial electrostatic potentials φ(i) (i = 1,...,L, here L is number of total sites), we first make two sweeps for warming before beginning the selfconsistent calculations for the longrange Coulomb interactions. Then, for the next 10 sweeps, the electrostatic potentials φ(i) are updated by solving Poisson s equation [Eq. (2)] at each sweep. In general, the convergence of the selfconsistent procedure is very slow. Therefore, here we perform an extrapolation of φ(i) for each i, using the values calculated during those 10 sweeps, to an infinite number of sweeps. By comparing fully selfconsistent calculations, we have found that generally this extrapolation scheme gives a reasonable results. Finally, the obtained potential φ(i) is plugged back in Eq. (1), and 8 more sweeps are performed to calculate the ground state. The results reported below are obtained by retaining M =350 states, and the truncation error in the worst case is of order All DMRG calculations are done at T = 0, and J H =36 is used. 12 As a check of our DE model code, we have compared the case of a total zprojection of the spin S z = S max =26, on a lattice of L=32 sites and with a total number of conduction electrons N = 20, with the results of the spinless fermion model which is computed with a previously prepared DMRG code for the Hubbard model, 19 written completely independently from the present DE code. The potential φ(i) added in the spinless fermion calculation is the one extracted from the DE run. The differences in energies are found to be of order To study transport properties, the timedependent DMRG technique is used. 20 The electrostatic potentials φ(i) are fixed to the ones obtained above, and a small bias potential V =0.01 is applied at time t=0, which triggers a timeevolution of the system. 21 The bias potential is applied only on a few sites at the edges of the system, and the current as a function of t is measured on the two links connecting the central region to the two outer portions of the system. The amplitude of J(t), defined as the average of these two currents, scales approximately linearly with the number of sites on which the bias potential V is applied. As it is well known, 21 J(t) follows an oscillatory evolution with time due to the open boundary conditions used in the DMRG process (electrons cannot leave the system). Thus, to obtain a measure of the conductance, the average of J(t)/ V over
5 5 the first halfperiod of the oscillation is considered. 21 III. RESULTS AT ZERO TEMPERATURE In this section, the main results obtained in our numerical simulations will be described. A. Allmanganite trilayer geometry using classical t 2g spins 1. Even number of sites in the barrier Figure 2 shows the zerotemperature optimization results corresponding to a 1D trilayer geometry [Fig. 1 (a)] consisting of 20 sites in each lead, and 4 sites in the middle. The positive charge, regulated by n +, is 0.65 at each lead and 1.0 in the middle (in e=1 units). The strength of the longrange Coulomb interaction is chosen as α=1.0. Figure 2(a) shows the converged local electronic density n(i) vs. the site location i, along the 44 sites chain. In the leads, the electronic density closely matches the expected result The oscillations at the end of the chain near i=1 and 44 are due to Friedel oscillations. In the 4sites center, 2 of the sites have n(i) very close to 1, while the other 2 have a smaller density due to the chargetransfer effect of the longrange forces. The overall electronic density profile is reasonable and in agreement with qualitative expectations. The lower panel Fig. 2(b) contains the most important result for this particular geometry. There, the orientations of the classical t 2g spins are shown via the spherical coordinates angle ϕ, as a function of position i. Note first that each lead has classical t 2g spins polarized in a ferromagnetic state, namely all sites have approximately the same ϕ, as expected from the wellknown doubleexchange mechanism. 22 This ferromagnetism at the leads is compatible with phase diagrams gathered in previous studies. 12 However, in the near absence of magnetic fields, h ext = , the angle ϕ of the two ferromagnetic leads differs by π, signaling an antiparallel arrangement of magnetic moments between the two ferromagnetic leads (the tiny field was used simply to orient the spins along a direction which simplifies the discussion, and it does not have any other important effect). This antiparallelism is in excellent agreement with the expected results based on the introductory discussion: if the number of sites in the antiferromagnetic barrier is even, then an antiparallel orientation of ferromagnetic moment between the leads should occur. In the barrier region, the classical spins are arranged in an antiferromagnetic pattern, since there n(i) 1 and an antiferromagnetic spin orientation is preferred. 12 The results become even more interesting as the magnetic field is increased. In this case, the relative orientation of the ferromagnetic moments in the leads changes very rapidly, as shown in Fig. 2(b). For fields as small n(i) ϕ/π (a) (b) h//x, θ~π/2 =0.0 =0.005 = = = =0.001 = FIG. 2: (Color online) (a) Local electron density n(i) and (b) classical spin orientation S i = (θ i, ϕ i) (0 θ i π, 0 ϕ i 2π) in spherical coordinates vs. site location i, on a trilayer chain with L (L) = L (R) = 20 sites in each lead and L (C) = 4 sites in the center. The 1D DE model with J H=8.0 and α=1.0 is used, and the results are obtained via an optimization method at zero temperature. Lead s positive background charge is n (L) + =n(r) + =0.65, and a central positive background charge is n (C) + =1.0. A magnetic field is applied in the direction opposite to xdirection (x), and the magnitude (h ext) is shown in the figures. In (b), θ i π/2 for all h ext s. As h ext increases, the spins gradually rotate toward x in the xy plane, and finally they align ferromagnetically. The positions of the two interfaces are denoted by vertical dashed lines. as h ext =0.005 (in units of the hopping t), the magnetic moments of the ferromagnetic leads are already nearly aligned. As shown below, this produces drastic changes in the conductance of the ensemble. Results for intermediate values of the magnetic field, also in Fig. 2(b), show that the transition from antiparallel to parallel orientation of the ferromagnetic lead s moments is smooth and, moreover, noticeable changes can be observed even for fields as tiny as h ext = (a discussion of how small this field is in physical units is below). The relative orientation of the magnetic moments of the leads, and their rotation with magnetic fields, induce substantial modifications in the conductance and a concomitant large magnetoresistance. Figure 3(a) shows the conductance of the trilayer vs. magnetic field h ext. At fields zero or very small, the antiparallel orientation of the lead s moments produces a very small conductance. This is reasonable since the spin orientation which can conduct in one lead, is blocked by the antiparallel lead. However, as h ext increases, there are substantial changes in the conductance. For fields as small as h ext =0.0002, the conductance has changed by about 3 orders of magnitude already, at least for the particular system studied here. Note that if t is assumed to be i
6 6 0.1 ev, then h ext = is approximately 0.1 T. The conductance increases further, by more than an order of magnitude, by increasing h ext toward the value where the moments of the leads become essentially parallel. The conductances remain in absolute value much smaller than the perfect conductance 2e 2 /h (h: Planck constant), but its relative changes can be large, as illustrated in Fig. 3(b). In the widely used definition for conductance changes, which has the zero field conductance in the denominator, the magnetoresistance ratio can be very large, and it reaches almost 200,000% at h ext = G(h ext )/(2e 2 /h) [G(h ext )G(105 )]/G(105 ) (a) (b) h ext FIG. 3: (Color online) (a) Conductance G(h ext) in units of 2e 2 /h (h: Planck constant) and (b) magnetoresistance (MR) ratio, as a function of an applied magnetic field h ext. The results are calculated for the 1D DE model with J H=8.0, α=1.0, and T=0.0. Positive background charges are n (L) + =n(r) + =0.65 and n(c) + =1.0, and leads and central region sizes are L (L) =L (R) =20 and L (C) =4, respectively. To estimate the MR ratio, defined in the vertical axis of (b), G(h ext) with h ext = 10 5, instead of G(h ext = 0), is used since the conductance at h ext=0 vanishes. Note that with increasing h ext the conductance G(h ext), and the MR ratio, increases almost linearly except for very small h ext ( < ). To give a better perspective of the importance of these numbers, note that in a recent numerical study 23 of the same model used for the trilayer geometry but defined on a finite twodimensional cluster without interfaces, the CMR phenomenon was observed for larger magnetic fields h ext =0.05. In this case the MR magnitude was 10,000% at the best. Thus, the trilayer geometry investigated here certainly produces a more dramatic effect at smaller fields than in the bulk simulations. To help experimental readers who are more used to resistance plots, in Fig. 4(a), the resistance R of the trilayer with an even number of sites in the barrier is shown as a function of magnetic field h ext. Notice the rapid change in R at small h ext, which is the main result of this paper. In experimental similar plots, such as those reported for STO and LAO as barriers, hysteresis loops are often observed in TMR vs. h ext, and moreover the effects at tiny fields are negligible. 6,7,10 These differences are caused by the anisotropies present in real experiments due to strain in the samples, as briefly explained in Sec. IC, effect that has been mainly neglected in our calculations (with the exception of the results shown in Fig. 15 below). In Fig. 4(b), magnetization M of the classical t 2g spins for the trilayer ensemble vs. h ext is shown. Compatible with the spin arrangements already described, there is no net magnetization M at h ext =0, since the contributions of the ferromagnetic leads cancel out. However, with increasing h ext, there is a rapid increase in M because the lead s magnetic moments are aligning in the same direction. The subsequent small increases in M and decrease in R, say for h ext =0.001 or larger, are due to further fine alignment of the spins close to the central region (the spin orientation in the central region remains antiferromagnetic, which eventually turns to FM with much larger h ext ). Thus, the effective height of the barrier melts as h ext (or T, as discussed in the next section) increases in this system. G 1 (2e 2 /h) M/M S (a) (b) h ext FIG. 4: (Color online) (a) Resistance (inverse of conductance) vs. magnetic field h ext for an even number of sites L (C) =4 in the central barrier at zero temperature. The leads each has L (L) =L (R) =20 sites, and the positive background charges are n (L) + =n(r) + =0.65 and n(c) + =1.0 in the leads and central region, respectively. The couplings used are J H=8.0, and α=1.0. Notice that the large changes in resistance occur at very small magnetic fields. (b) Total magnetization M of the classical t 2g spins vs. h ext, indicating the rapid development with h ext of a net magnetization. M S is the maximum possible magnetization. 2. Odd number of sites in the barrier The numerical results obtained for the case of an odd number of sites in the barrier are very different from those reported thus far. In Fig. 5, the results for the case of L (C) = 5 sites in the barrier are reported. Fig. 5 (a) shows the electronic density n(i) vs. i, which is similar
7 7 to the results for the case of L (C) = 4 sites in the barrier [Fig. 2 (a)]. The electrostatic potential for electrons φ(i), caused by the longrange Coulomb interactions, shown in Fig. 5 (b), is also canonical: in the central region more electrons are expected to accumulate since there n + (i) is larger than in the leads. The important qualitative difference with the previous results in Sec. III A1 is presented in Fig. 5 (c). Here, the spin correlation functions for the classical t 2g spins indicate that the magnetic moments of the leads are parallel to each other, even in the absence of magnetic fields. This is in agreement with the qualitative scenario for these geometries described in the introduction (Sec. I B). As a consequence, the case of an odd number of sites in the barrier does not present the same huge magnetoresistance at small magnetic fields as for the even case. 1.0 n(i) φ(i) <S i S 11 > (a) (b) (c) : T=0.01 : T= FIG. 5: (Color online) (a) Local electron density n(i), (b) electrostatic potential φ(i), and (c) classical t 2g spin correlation function S i S j from the central site at j=11. The Monte Carlo techniques and optimization method are used for the 1D DE model with J H=8.0 and α=2.0 at T=0.01 and T = 0, respectively. The positive background charges are n (L) + =n(r) + =0.625 and n(c) + =1.0, and the system size used is L (L) =L (R) =8 and L (C) =5. Here, φ(i) is selfconsistently determined. The interface positions are denoted by vertical dashed lines. The resistance R vs. magnetic field h ext is shown in Fig. 6(a). As in the case of the even L (C), clearly R decreases with increasing h ext. However, the scales involved are very different. While for L (C) even, there are huge changes at h ext as small as (Fig. 4), for the L (C) odd case the resistance remains almost the same up to h ext =0.02. The reason is that the magnetic field does not need to align the magnetic moments of the leads in this case (they are already aligned), and moreover the i updownup arrangement of the central region is compatible with the parallel leads moments. The only modification needed in the spin arrangement is the correction in the orientation of the central spins that are pointing the wrong way. This process takes place between fields h ext =0.02 and 0.05 approximately. After that, the entire system is ferromagnetic and the resistance remains constant. For completeness, Fig. 6(b) shows the total magnetization of the classical t 2g spins. As expected, initially, M is very robust, and it becomes saturated at h ext G 1 (2e 2 /h) M/M S (a) (b) h 0.1 ext FIG. 6: (Color online) (a) Resistance (inverse of conductance) vs. magnetic field h ext for an odd number of sites L (C) =5 in the central barrier at T=1/800. The leads have L (L) =L (R) = 8 sites, and the positive background charges are n (L) + =n(r) + =0.625 and n(c) + =1.0 for the leads and central region, respectively. The couplings used are J H=8.0 and α=1.0. (b) Total magnetization M of the classical t 2g spins vs. magnetic field h ext, indicating that the system is overall ferromagnetic at all magnetic fields. M S is the maximum possible magnetization. φ(i) is determined selfconsistently at T =0.2 and h ext = 0, and then used for other temperatures and h ext (see more details in the text). B. Allmanganite trilayer geometry using quantum t 2g spins The existence of parallel or antiparallel arrangements of the magnetic moments in the left and right leads is also investigated for the 1D DE model with quantum localized t 2g spins S i [Eq. (1)] at T = 0 by the DMRG technique. For numerical simplicity, spin1/2 is employed, instead of the realistic value 3/2. In Fig. 7, the (zcomponent) spin correlation functions Si zsz j are reported for a typical set of parameters, choosing one of the centralregion spins (j = 0) as a reference. There are 4 and 5 sites in the central region in Fig. 7 (a) and (b), respectively. In the case of even number of central sites [Fig. 7 (a)], at least for large values of α such as 2, the antiferromagnetic spin correlations
8 8 in the central region are clearly observed, and moreover the magnetic moments of the left and right leads tend to align antiparallel. However, quantum fluctuations, enhanced by the spin1/2 and onedimensionality nature of the model, make the spin correlations at longer distances weaker, and the correlations become very small for i > 4. Similarly, quantum fluctuations reduce spin correlations at large distances also for odd number of central sites, shown in Fig. 7 (b). However, in this case, a tendency of parallel alignment of the magnetic moments between the left and right leads can still be observed. Thus, overall features observed in the case of quantum t 2g spins are in good qualitative agreement with the ones observed in the classical t 2g spin case. Realistic twoor threedimensional manganite trilayers are expected to behave more similarly to the classical t 2g spin case than the quantum spin1/2 onedimensional case, where the quantum fluctuations are the strongest. In fact, quantum fluctuations appear detrimental for the performance of the device proposed in this paper. Higher dimensional arrangements will have a stronger tendency to spin order, as the classical spins do here.
9 9
10 10 tions have the opposite sign (minus) as compared to the ones without the barrier. This is simply because in this trilayer case there is an even number of sites in the central region, and therefore the magnetic moments between the leads align antiferromagnetically (Sec. III). Here the calculations are carried out by first obtaining the electrostatic potential φ(i) at high temperature, where the spins are not ordered, and then keeping this potential the same as the temperature is reduced. This procedure considerably alleviates the numerical effort, particularly regarding the Poisson s equation iterations, and tests in small systems have shown that this trick does not alter the results qualitatively. As also seen in Fig. 10, the spin correlation functions obtained by this method have a relatively minor dependence with α. The main point to remark is that these spin correlations become negligible at a temperature T 0.01, which is considerably smaller than the relevant temperature of the pure ferromagnetic system without the barrier. As a consequence, it is clear that a strong similarity with previous experimental results for STO barriers 6 may exist in this case. Expressed qualitatively, our results indicate that there is a temperature scale T, much smaller than the critical temperature T C, where the orientation of the leads magnetic moments ceases to be antiferromagnetic. As shown below, this is correlated with important changes in the magnetoresistance effect. In fact, the large MR effect at low temperature seems to occur due to the existence of an effective coupling J eff which produces the antiparallel alignment of the leads magnetic moments. This is reasonable, since J eff is an effective weak coupling across a tunneling insulating barrier. When the temperature is of the order of this coupling or larger, the antiparallel arrangement is no longer preferable and in our model the leads moments rotate freely with respect to one another. A systematic study of the influence of the size of the central region L (C) on the classical t 2g spin correlations between the leads is reported in Figure 11. As expected (Sec. IB), for L (C) even (odd) these spin correlations are negative (positive) at low temperatures, indicating strong antiferromagnetic (ferromagnetic) correlations between the ferromagnetic leads moments. The magnitude of this correlation decreases as L (C) increases, in agreement with the expected reduction of the effective coupling J eff discussed above. Thus, the thinner the barrier is, the better the temperature effects become in the trilayer geometry proposed here, namely the higher T is. Our discussion thus far has been based on the spin correlations at finite temperatures. It was concluded that the large resistance caused by the antiparallel configuration of the ferromagnetic leads moments does not survive all the way to the ferromagnetic critical temperatures of the leads. This is indeed observed in Fig. 12, where at T the MR effect is reduced to zero at fields such as h ext = , while at zero temperature [Fig. 3 (b)] the MR effect was huge at the same fields. However, even though the MR effect is truly enormous at very low temperature, at higher temperatures it is not negligi <S 5 S 12+L (C)> L=8+L (C) +8, N + =5+L (C) +5 φ(x): fixed at T=1/5 : L (C) =3 : L (C) =4 : L (C) =5 : L (C) =6 : L (C) =7 : L (C) = T 1 FIG. 11: (Color online) Classical t 2g spin correlation functions S i S j between sites i=5 (belonging to the left lead) and site j=12+l (C) (belonging to the right lead), for the 1D DE model with J H=8.0, α=1.0, n (L) + =n(r) + =0.625, n(c) + =1.0, L (L) =L (R) =8, and L (C) =3,4,,8. Here, φ(i) is determined selfconsistently at T =0.2 and then used for other temperatures. ble, at least in the several Teslas scale of magnetic fields h ext. For example, in Fig. 12, the MR ratio is plotted vs. temperature, for different values of h ext. Note that [G(h ext ) G(0)]/G(0) is the same as the more standard definition [R(0) R(h ext )]/R(h ext ), where the resistance R(h ext )=1/G(h ext ). For fields such as h ext =0.02 and 0.03 corresponding to 20 and 30 T, respectively, if it is assumed t 1,000 T the MR ratio can be as large as 100 or 500% at temperatures of the order of T C /2. In the calculations described so far, no easy axis has been chosen. In other words, no anisotropies were introduced. However, the introductory discussion suggests that many materials, particularly when in thinfilm form, do have an easy axis mainly due to the influence of the substrate (Sec. I C). If due to this effect the magnetic moments of the leads cannot rotate freely with respect to one another as isotropic Heisenberg vectors, but are pointing along a particular direction as Ising variables, the temperature scale T above which the magnetic moments of the leads become uncorrelated should increase: Heisenberglike isotropic spins can be disordered by thermal fluctuations more easily than Isinglike spins. On the other hand, making more rigid the antiparallel magnetic connection between the leads moments will also prevent their alignment in very small magnetic fields: larger magnetic fields may be needed to achieve the same effect as before, i.e., large MR effect. These competing tendencies will be discussed in more detail below. To investigate this issue, extra couplings between classical t 2g spins are added to the model, as shown in Fig. 13. Via direct Heisenberg couplings between the classical spins, J AF (antiferromagnetic) and J F (ferromagnetic),
11 [G(h ext )G(0)]/G(0) (%) =0.001 =0.003 =0.005 =0.01 =0.02 = T <S 5 S 16 > Uniform (L=20, N=12) L=8+4+8, N + =5+4+5 φ(x): fixed at T=1/5 : J AF =J F =0.0 : J AF =0.1, J F =0.0 : J AF =J F = T 1 FIG. 12: (Color online) Temperature dependence of the MR ratio [(G(h ext) G(0))/G(0)] 100 for the 1D DE model with J H=8.0, α=1.0, n (L) + =n (R) + =0.625, n (C) + =1.0, L (L) =L (R) =8, and L (C) =4. Applied magnetic fields h ext are indicated in the figure. φ(i) is determined selfconsistently at T =0.2 and used for the other temperatures. Note that the effect reported at T=0 in Fig. 3 is much larger in magnitude of the order of 200,000% at h ext=0.002 (in that figure the factor 100 was not used as in here). In the range of temperatures shown in this figure, the original T =0.0 nearly perfect antiferromagnetic alignment of the leads magnetic moments is already lost at h ext=0, and thus the changes in resistances are not as dramatic as observed at T = 0. FIG. 14: (Color online) Classical t 2g spin correlation functions S i S j between site i = 5 (belonging to the left lead) and site j = 16 (belonging to the right lead), as a function of temperature T. Monte Carlo simulations are used for the 1D DE model with J H=8.0 and α = 1.0. The positive background charge densities are n (L) + =n (R) + = and n (C) + = 1.0, and the cluster used is L (L) = L (R) = 8 and L (C) = 4. The results with J AF = J F = 0.1 are shown by triangles, and the results with J AF = 0.1 but no J F are denoted by diamonds. For comparison, the results for a uniform DE model without the barrier (circles) and the results with the central barrier but no J AF and J F (squares) are also plotted. These are reproduced from Fig. 10. Note that with nonzero J F and J AF, the spin correlations now vanish at almost the same temperature as in the case without the barrier (circles). Here, φ(i) is determined selfconsistently at T=0.2 and is subsequently used for other lower temperatures. J F J AF J AF J AF J F FIG. 13: (Color online) Schematic representation of the 1D DE model [Eq. (1)] for a LSMO/LMO/LSMO trilayer (see also Fig. 1) with additional Heisenberg couplings between classical t 2g spins, which are introduced to simulate anisotropies. Antiferromagnetic J AF, as well as ferromagnetic J F, couplings are added only in the central region and the bonds connecting to the central region, as indicated in the figure. The two interface positions are denoted by vertical dashed lines. both the antiferromagnetic spin arrangement in the central region and the coupling between the center and the leads can be made more rigid. That this procedure helps regarding the T problem is clear in Fig. 14 where the classical t 2g spin correlation functions are shown. Contrary to the case of weakly coupled leads, now a robust spin correlation between them survives up to T C. However, the MR effect is not improving at very small fields (see Fig. 15). On the contrary, larger values of h ext are needed to achieve the same MR effect as before (for instance, the MR ratio at h ext =0.01 without anisotropies is 3000% at T 0.001, while it is 1500% here with anisotropy). Thus, as already mentioned briefly, the overall conclusion is that there are two competing tendencies to consider in these investigations: (i) on one hand, a weak coupling among the leads, mediated by the central region, is needed in order for a tiny magnetic field to cause a huge effect in transport; (ii) on the other hand, for the same reason, a small temperature can entirely wash out the effect. Adding anisotropies increases the effective coupling between the leads magnetic moments, thus helping with the temperature issue (ii), but reciprocally, larger magnetic fields are needed to achieve the same MR effect. Investigating the subtle balance between these competing tendencies is a great challenge, both for theorists and experimentalists.
12 12 [G(h ext )G(0)]/G(0) (%) =0.001 =0.005 =0.01 =0.02 =0.03 =0.05 n(i) : V m =2 : V m = T=1/800 : V m =6 : V m = : V m = i FIG. 15: (Color online) The same as in Fig. 12 except that additional couplings between the classical t 2g spins, J AF=J F=0.1, are added to simulate the presence of anisotropies (see Fig. 13). The applied magnetic fields h ext are indicated in the figure. The electrostatic potential φ(i) is determined selfconsistently at T =0.2 and then used for other lower temperatures. T FIG. 16: (Color online) Electron density n(i) for the 1D LSMO/STO/LSMO model (see the text) with J H = 8.0 and α = 1.0, at T = 1/800, and for various values of V m (indicated in the figure). The positive background charges are n (L) + =n (R) + =0.625 and n (C) + =0.0, and the system size studied is L (L) =L (R) =8 and L (C) =4. The positions of the two interfaces are denoted by vertical dashed lines. The electrostatic potential φ(i) is determined selfconsistently. V. TIOXIDE BARRIER Although the focus of our effort has been on the LSMO/LMO/LSMO trilayer, as mentioned in the introduction we have also carried out model Hamiltonian simulations for the more standard case of a nonmagnetic insulator as a barrier. A widely studied material for this purpose is STO, which is here mimicked simply by a tightbinding Hamiltonian for the barrier, with its energy levels shifted by a oneparticle site potential V m which controls the height of the barrier. In this section, results for the case LSMO/STO/LSMO are briefly discussed, with the emphasis on qualitative aspects and comparisons with the case of LMO as barrier. The details of the model Hamiltonian were already described in Sec. II, and the technique employed is the MC simulation. Once again, it should be remarked that subtle effects such as dead layers are not considered in this study (Sec. I C), and their presence may affect quantitatively our conclusions. The local electronic density n(i) is reported in Fig. 16 for the 1D LSMO/STO/LSMO model with different values of the site potential V m in the central region. It is observed that n(i) in the central region gradually increases from nearly zero to 0.4 with decreasing V m, indicating that the barrier hight decreases with V m, and consequently the effective coupling between the leads becomes stronger. Note that the lower band of the lead (described by the DE model) is centered at J H, and thus the band of the central region and the lower band of the lead are perfectly aligned (i.e., zero barrier height) when V m = J H (and α = 0). In Fig. 17, the MR ratio vs. temperature for the case V m = 7.0 is shown. Notice that the MR effect becomes appreciable at temperatures comparable to the Curie temperature of the individual ferromagnetic leads. This is qualitatively similar to the effect observed in LSMO/LMO/LSMO for the case where an anisotropy was introduced (Fig. 15), which effectively caused a stronger effective coupling between the magnetic moments of the left and right leads. Thus, it appears that the value V m = 7.0 chosen for this example allows for a robust leftright coupling (as also expected from n(i) shown in Fig. 16), concomitant with the survival of a large MR effect up to the Curie temperature. It is also observed in Fig. 17 that because of the strong effective coupling between the leads, the MR ratio for small magnetic fields ( < 0.003) is not as large as in the case of the small effective coupling discussed below (Fig. 18). Figure 18 shows results for the same parameters as in Fig. 17, but simply making the height of the barrier V m much larger, i.e., the left and right leads being nearly decoupled. Three effects are obvious to the eye: (i) the large MR effect appears now at lower temperatures. For example, in Fig. 18 the MR becomes nonzero at T 0.02, while in Fig. 17 the same occurred at a higher temperature (ii) On the other hand, increasing the height of the barrier much increases the MR ratio at low temperatures and small magnetic fields. For example, in Fig. 18 the MR ratio is about 1,000% at T and h ext = 0.001, while in Fig. 17 it is about 200% at the same T and h ext. This occurs because the barrier is so large in Fig. 18 that in the absence of magnetic fields, the magnetic moments of the left and right leads are almost decoupled, and thus applying a very small magnetic field is enough to align the leads magnetic moment and
MAGNETORESISTANCE PHENOMENA IN MAGNETIC MATERIALS AND DEVICES. J. M. De Teresa
MAGNETORESISTANCE PHENOMENA IN MAGNETIC MATERIALS AND DEVICES J. M. De Teresa Instituto de Ciencia de Materiales de Aragón, Universidad de ZaragozaCSIC, Facultad de Ciencias, 50009 Zaragoza, Spain. Email:
More information(a) (b) Supplementary Figure 1. (a) (b) (a) Supplementary Figure 2. (a) (b) (c) (d) (e)
(a) (b) Supplementary Figure 1. (a) An AFM image of the device after the formation of the contact electrodes and the top gate dielectric Al 2 O 3. (b) A line scan performed along the white dashed line
More informationCurrentdriven Magnetization Reversal in a Ferromagnetic Semiconductor. (Ga,Mn)As/GaAs/(Ga,Mn)As Tunnel Junction
Currentdriven Magnetization Reversal in a Ferromagnetic Semiconductor (Ga,Mn)As/GaAs/(Ga,Mn)As Tunnel Junction D. Chiba 1, 2*, Y. Sato 1, T. Kita 2, 1, F. Matsukura 1, 2, and H. Ohno 1, 2 1 Laboratory
More informationTesting the Monte Carlo  Mean Field approximation in the oneband Hubbard model
Testing the Monte Carlo  Mean Field approximation in the oneband Hubbard model Anamitra Mukherjee 1, Niravkumar D. Patel 1, Shuai Dong 2, Steve Johnston 1, Adriana Moreo 1,3, and Elbio Dagotto 1,3 1
More informationμ (vector) = magnetic dipole moment (not to be confused with the permeability μ). Magnetism Electromagnetic Fields in a Solid
Magnetism Electromagnetic Fields in a Solid SI units cgs (Gaussian) units Total magnetic field: B = μ 0 (H + M) = μ μ 0 H B = H + 4π M = μ H Total electric field: E = 1/ε 0 (D P) = 1/εε 0 D E = D 4π P
More informationSpontaneous Symmetry Breaking
Spontaneous Symmetry Breaking Second order phase transitions are generally associated with spontaneous symmetry breaking associated with an appropriate order parameter. Identifying symmetry of the order
More informationarxiv:condmat/ v1 [condmat.strel] 4 Sep 2002
arxiv:condmat/0209089v1 [condmat.strel] 4 Sep 2002 Double exchange and orbital correlations in electron doped manganites Tulika Maitra 1 and A. Taraphder 2 Department of Physics & Meteorology and Centre
More informationUniversal valenceband picture of. the ferromagnetic semiconductor GaMnAs
Universal valenceband picture of the ferromagnetic semiconductor GaMnAs Shinobu Ohya *, Kenta Takata, and Masaaki Tanaka Department of Electrical Engineering and Information Systems, The University of
More informationSpins and spinorbit coupling in semiconductors, metals, and nanostructures
B. Halperin Spin lecture 1 Spins and spinorbit coupling in semiconductors, metals, and nanostructures Behavior of nonequilibrium spin populations. Spin relaxation and spin transport. How does one produce
More informationLab 70 in TFFM08. Curie & Ising
IFM The Department of Physics, Chemistry and Biology Lab 70 in TFFM08 Curie & Ising NAME PERS. NUMBER DATE APPROVED Rev Aug 09 Agne 1 Introduction Magnetic materials are all around us, and understanding
More informationarxiv: v1 [condmat.strel] 11 Nov 2013
arxiv:1311.2420v1 [condmat.strel] 11 Nov 2013 MonteCarlo simulation of graphene in terms of occupation numbers for the ecitonic order parameter at heagonal lattice. Institute for Theoretical Problems
More informationThe Oxford Solid State Basics
The Oxford Solid State Basics Steven H. Simon University of Oxford OXFORD UNIVERSITY PRESS Contents 1 About Condensed Matter Physics 1 1.1 What Is Condensed Matter Physics 1 1.2 Why Do We Study Condensed
More informationCorrelations between spin accumulation and degree of timeinverse breaking for electron gas in solid
Correlations between spin accumulation and degree of timeinverse breaking for electron gas in solid V.Zayets * Spintronic Research Center, National Institute of Advanced Industrial Science and Technology
More informationThe Hubbard model for the hydrogen molecule
INSTITUTE OF PHYSICS PUBLISHING Eur. J. Phys. 3 (00) 11 16 EUROPEAN JOURNAL OF PHYSICS PII:S01430807(0)3516 The Hubbard model for the hydrogen molecule B AlvarezFernández and J A Blanco Dpto. de Física,
More informationAn introduction to magnetism in three parts
An introduction to magnetism in three parts Wulf Wulfhekel Physikalisches Institut, Karlsruhe Institute of Technology (KIT) Wolfgang Gaede Str. 1, D76131 Karlsruhe 0. Overview Chapters of the three lectures
More informationTime Resolved Faraday Rotation Measurements of Spin Polarized Currents in Quantum Wells
Time Resolved Faraday Rotation Measurements of Spin Polarized Currents in Quantum Wells M. R. Beversluis 17 December 2001 1 Introduction For over thirty years, silicon based electronics have continued
More informationComplexity in Transition Metal Oxides
Complexity in Transition Metal Oxides Adriana Moreo Dept. of Physics and ORNL University of Tennessee, Knoxville, TN, USA. Supported by NSF grants DMR0443144 and 0454504. Collaborators G. Alvarez (ORNL)
More informationSIMULATIONS ON DILUTE MAGNETIC SEMICONDUCTOR PROPERTIES
Romanian Reports in Physics, Vol. 62, No. 1, P. 115 120, 2010 SIMULATIONS ON DILUTE MAGNETIC SEMICONDUCTOR PROPERTIES M. NEGOITA, E. A. PATROI, C. V. ONICA National Institute for Research and Development
More informationThe exchange interaction between FM and AFM materials
Chapter 1 The exchange interaction between FM and AFM materials When the ferromagnetic (FM) materials are contacted with antiferromagnetic (AFM) materials, the magnetic properties of FM materials are drastically
More informationMetropolis Monte Carlo simulation of the Ising Model
Metropolis Monte Carlo simulation of the Ising Model Krishna Shrinivas (CH10B026) Swaroop Ramaswamy (CH10B068) May 10, 2013 Modelling and Simulation of Particulate Processes (CH5012) Introduction The Ising
More informationPart III: Impurities in Luttinger liquids
Functional RG for interacting fermions... Part III: Impurities in Luttinger liquids 1. Luttinger liquids 2. Impurity effects 3. Microscopic model 4. Flow equations 5. Results S. Andergassen, T. Enss (Stuttgart)
More informationResearch Highlights. Salient results from our group. Mixed phosphides in SnP and SnMnP systems
Research Highlights Dilute magnetic semiconductors and Spintronics Spintronics is a branch of electronics emerged from the dilute magnetic semiconductor in an aspect of utilization of the spin in addition
More informationChapter 3 Properties of Nanostructures
Chapter 3 Properties of Nanostructures In Chapter 2, the reduction of the extent of a solid in one or more dimensions was shown to lead to a dramatic alteration of the overall behavior of the solids. Generally,
More informationXRay Magnetic Dichroism. S. Turchini ISMCNR
XRay Magnetic Dichroism S. Turchini SMCNR stefano.turchini@ism.cnr.it stefano.turchini@elettra.trieste.it Magnetism spin magnetic moment direct exchange: ferro antiferro superexchange 3d Ligand 2p 3d
More informationExchange interactions
Exchange interactions Tomasz Dietl Institute of Physics, Polish Academy of Sciences, PL02668Warszawa, Poland Institute of Theoretical Physics, University of Warsaw, PL00681Warszawa, Poland 1. POTENTIAL
More informationSTM and graphene. W. W. Larry Pai ( 白偉武 ) Center for condensed matter sciences, National Taiwan University NTHU, 2013/05/23
STM and graphene W. W. Larry Pai ( 白偉武 ) Center for condensed matter sciences, National Taiwan University NTHU, 2013/05/23 Why graphene is important: It is a new form of material (two dimensional, single
More informationGiant Magnetoresistance
GENERAL ARTICLE Giant Magnetoresistance Nobel Prize in Physics 2007 Debakanta Samal and P S Anil Kumar The 2007 Nobel Prize in Physics was awarded to Albert Fert and Peter Grünberg for the discovery of
More informationCoaxial cable. Coaxial cable. Magnetic field inside a solenoid
Divergence and circulation Surface S Ampere s Law A vector field is generally characterized by 1) how field lines possibly diverge away from or converge upon (point) sources plus 2) how field lines circulate,
More informationarxiv:condmat/ v1 [condmat.strel] 21 Mar 2006
NonFermiliquid phases in the twoband Hubbard model: Finitetemperature exact diagonalization study of Hund s rule coupling A. Liebsch and T. A. Costi Institut für Festkörperforschung, Forschungszentrum
More informationLecture 24 Origins of Magnetization (A number of illustrations in this lecture were generously provided by Prof. Geoffrey Beach)
Lecture 4 Origins of Magnetization (A number of illustrations in this lecture were generously provided by Prof. Geoffrey Beach) Today 1. Magnetic dipoles.. Orbital and spin angular momenta. 3. Noninteracting
More informationExchange bias in core/shell magnetic nanoparticles: experimental results and numerical simulations
Exchange bias in core/shell magnetic nanoparticles: experimental results and numerical simulations Xavier Batlle, A. Labarta, Ò. Iglesias, M. García del Muro and M. Kovylina Goup of Magnetic Nanomaterials
More informationFerromagnetism and Anomalous Hall Effect in Graphene
Ferromagnetism and Anomalous Hall Effect in Graphene Jing Shi Department of Physics & Astronomy, University of California, Riverside Graphene/YIG Introduction Outline Proximity induced ferromagnetism Quantized
More informationThe 1+1dimensional Ising model
Chapter 4 The 1+1dimensional Ising model The 1+1dimensional Ising model is one of the most important models in statistical mechanics. It is an interacting system, and behaves accordingly. Yet for a variety
More informationMomentumspace and Hybrid Real Momentum Space DMRG applied to the Hubbard Model
Momentumspace and Hybrid Real Momentum Space DMRG applied to the Hubbard Model Örs Legeza Reinhard M. Noack Collaborators Georg Ehlers Jeno Sólyom Gergely Barcza Steven R. White Collaborators Georg Ehlers
More informationEXCHANGE INTERACTIONS: SUPEREXCHANGE, DOUBLE EXCHANGE, RKKY; MAGNETIC ORDERS. Tomasz Dietl
Analele Universităţii de Vest din Timişoara Vol. LIII, 2009 Seria Fizică EXCHANGE INTERACTIONS: SUPEREXCHANGE, DOUBLE EXCHANGE, RKKY; MAGNETIC ORDERS Tomasz Dietl Institute of Physics, Polish Academy
More informationMagnetic Oxides. Gerald F. Dionne. Department of Materials Science and Engineering Massachusetts Institute of Technology
Magnetic Oxides Gerald F. Dionne Department of Materials Science and Engineering Massachusetts Institute of Technology Spins in Solids Summer School University of Virginia Charlottesville, VA 21 June 2006
More informationPrinciples and Applications of Superconducting Quantum Interference Devices (SQUIDs)
Principles and Applications of Superconducting Quantum Interference Devices (SQUIDs) PHY 300  Junior Phyics Laboratory Syed Ali Raza Roll no: 2012100124 LUMS School of Science and Engineering Thursday,
More informationarxiv:condmat/ v1 [condmat.other] 5 Jun 2004
arxiv:condmat/0406141v1 [condmat.other] 5 Jun 2004 Moving Beyond a Simple Model of Luminescence Rings in Quantum Well Structures D. Snoke 1, S. Denev 1, Y. Liu 1, S. Simon 2, R. Rapaport 2, G. Chen 2,
More informationLuigi Paolasini
Luigi Paolasini paolasini@esrf.fr LECTURE 5: MAGNETIC STRUCTURES  Mean field theory and magnetic order  Classification of magnetic structures  Collinear and noncollinear magnetic structures.  Magnetic
More informationChapter 3. Magnetic Model. 3.1 Magnetic interactions
Chapter 3 Magnetic Model In this chapter, the micromagnetic model for the description of the magnetic properties of a laterally nanostructured film during growth is presented. The main physical idea of
More informationarxiv:condmat/ v1 [condmat.strel] 9 May 2001
Positively charged magnetoexcitons in a semiconductor quantum well. C. Riva and F. M. Peeters Departement Natuurkunde, Universiteit Antwerpen (UIA), B2610 Antwerpen, Belgium arxiv:condmat/0105192v1
More informationOptical Lattices. Chapter Polarization
Chapter Optical Lattices Abstract In this chapter we give details of the atomic physics that underlies the Bose Hubbard model used to describe ultracold atoms in optical lattices. We show how the ACStark
More information1 CHAPTER 12 PROPERTIES OF MAGNETIC MATERIALS
1 CHAPTER 12 PROPERTIES OF MAGNETIC MATERIALS 12.1 Introduction This chapter is likely to be a short one, not least because it is a subject in which my own knowledge is, to put it charitably, a little
More informationintroduction: what is spinelectronics?
Spindependent transport in layered magnetic metals Patrick Bruno MaxPlanckInstitut für Mikrostrukturphysik, Halle, Germany Summary: introduction: what is spinelectronics giant magnetoresistance (GMR)
More information1 The Heisenberg model
1 The Heisenberg model 1.1 Definition of the model The model we will focus on is called the Heisenberg model. It has the following Hamiltonian: H = 1 J ij S i S j. (1) 2 i,j i j Here i and j refer to sites
More informationSupplementary Figure 1 Experimental setup for crystal growth. Schematic drawing of the experimental setup for C 8 BTBT crystal growth.
Supplementary Figure 1 Experimental setup for crystal growth. Schematic drawing of the experimental setup for C 8 BTBT crystal growth. Supplementary Figure 2 AFM study of the C 8 BTBT crystal growth
More informationarxiv:condmat/ v1 [condmat.strel] 11 Aug 2003
Phase diagram of the frustrated Hubbard model R. Zitzler, N. ong, h. Pruschke, and R. Bulla Center for electronic correlations and magnetism, heoretical Physics III, Institute of Physics, University of
More informationE (MV cm 1 ) E // [001] x=0.7 E // [001] x=0.5. E // [001] E // [110] x=0.9. x=0.5
15 1 E // [1] x=.5 a E // [1] x=.7 b P (µc cm 2 ) 5 15 1 5 1 st cycle 2 nd cycle 3 rd cycle E // [1] E // [11] x=.9 x=.5 c d.5 1 1.5 2 2.5 3.5 1 1.5 2 2.5 3 E (MV cm 1 ) Supplementary Figure 1: The P
More informationEffects of spinorbit coupling on the BKT transition and the vortexantivortex structure in 2D Fermi Gases
Effects of spinorbit coupling on the BKT transition and the vortexantivortex structure in D Fermi Gases Carlos A. R. Sa de Melo Georgia Institute of Technology QMath13 Mathematical Results in Quantum
More informationPrinciples of Quantum Mechanics
Principles of Quantum Mechanics  indistinguishability of particles: bosons & fermions bosons: total wavefunction is symmetric upon interchange of particle coordinates (space,spin) fermions: total wavefuncftion
More informationChapter 4: Bonding in Solids and Electronic Properties. Free electron theory
Chapter 4: Bonding in Solids and Electronic Properties Free electron theory Consider free electrons in a metal an electron gas. regards a metal as a box in which electrons are free to move. assumes nuclei
More informationarxiv:condmat/ v1 [condmat.strel] 18 Oct 2002
Effect of SpinFlip Scattering on Electrical Transport in Magnetic Tunnel Junctions arxiv:condmat/0210393v1 [condmat.strel] 18 Oct 2002 ZhenGang Zhu, Gang Su, QingRong Zheng and Biao Jin Department
More information5. Semiconductors and PN junction
5. Semiconductors and PN junction Thomas Zimmer, University of Bordeaux, France Summary Learning Outcomes... 2 Physical background of semiconductors... 2 The silicon crystal... 2 The energy bands... 3
More informationSemiconductor Detectors are Ionization Chambers. Detection volume with electric field Energy deposited positive and negative charge pairs
1 V. Semiconductor Detectors V.1. Principles Semiconductor Detectors are Ionization Chambers Detection volume with electric field Energy deposited positive and negative charge pairs Charges move in field
More informationQuasiparticle dynamics and interactions in non uniformly polarizable solids
Quasiparticle dynamics and interactions in non uniformly polarizable solids Mona Berciu University of British Columbia à beautiful physics that George Sawatzky has been pursuing for a long time à today,
More informationMagnetism (FM, AFM, FSM)
Magnetism (FM, AFM, FSM) Karlheinz Schwarz Institute of Materials Chemistry TU Wien Localized vs. itinerant systems In localized systems (e.g. some rare earth) the magnetism is mainly governed by the atom
More informationElectric field control of magnetization using AFM/FM interfaces. Xiaoshan Xu
Electric field control of magnetization using AFM/FM interfaces Xiaoshan Xu Magnetoelectric effects α = μ 0 M E H M H = 0, E = 0 = 0 (General magnetoelectrics) M H = 0, E = 0 0, P H = 0, E = 0 0, (Multiferroics)
More informationA Study of the GroupIV Diluted Magnetic Semiconductor GeMn. Melissa Commisso Dolph Stu Wolf Group December 4 th, 2008
A Study of the GroupIV Diluted Magnetic Semiconductor GeMn Melissa Commisso Dolph Stu Wolf Group December 4 th, 2008 Outline Motivation and Background Our DMS : GeMn Hall Bars Summary / Future Work Motivation
More informationInterstitial Mn in (Ga,Mn)As: Hybridization with Conduction Band and Electron Mediated Exchange Coupling
Vol. 112 (2007) ACTA PHYSICA POLONICA A No. 2 Proceedings of the XXXVI International School of Semiconducting Compounds, Jaszowiec 2007 Interstitial Mn in (Ga,Mn)As: Hybridization with Conduction Band
More informationSurfaces, Interfaces, and Layered Devices
Surfaces, Interfaces, and Layered Devices Building blocks for nanodevices! W. Pauli: God made solids, but surfaces were the work of Devil. Surfaces and Interfaces 1 Interface between a crystal and vacuum
More informationReal Space Bogoliubov de Gennes Equations Study of the Boson Fermion Model
Vol. 114 2008 ACTA PHYSICA POLONICA A No. 1 Proceedings of the XIII National School of Superconductivity, L adek Zdrój 2007 Real Space Bogoliubov de Gennes Equations Study of the Boson Fermion Model J.
More informationContents. Acknowledgments
MAGNETIC MATERIALS Fundamentals and Applications Second edition NICOLA A. SPALDIN University of California, Santa Barbara CAMBRIDGE UNIVERSITY PRESS Contents Acknowledgments page xiii I Basics 1 Review
More informationThe Phase Transition of the 2DIsing Model
The Phase Transition of the 2DIsing Model Lilian Witthauer and Manuel Dieterle Summer Term 2007 Contents 1 2DIsing Model 2 1.1 Calculation of the Physical Quantities............... 2 2 Location of the
More informationMagnetism in correlatedelectron materials
Magnetism in correlatedelectron materials B. Keimer MaxPlanckInstitute for Solid State Research focus on delocalized electrons in metals and superconductors localized electrons: Hinkov talk outline
More informationIntroduction to Density Functional Theory
1 Introduction to Density Functional Theory 21 February 2011; V172 P.Ravindran, FMEcourse on Ab initio Modelling of solar cell Materials 21 February 2011 Introduction to DFT 2 3 4 Ab initio Computational
More information2.1 Experimental and theoretical studies
Chapter 2 NiO As stated before, the firstrow transitionmetal oxides are among the most interesting series of materials, exhibiting wide variations in physical properties related to electronic structure.
More informationElectronic Structure of Surfaces
Electronic Structure of Surfaces When solids made of an infinite number of atoms are formed, it is a common misconception to consider each atom individually. Rather, we must consider the structure of the
More informationTopological defects and its role in the phase transition of a dense defect system
Topological defects and its role in the phase transition of a dense defect system Suman Sinha * and Soumen Kumar Roy Depatrment of Physics, Jadavpur University Kolkata 70003, India Abstract Monte Carlo
More informationThe existence of a quantum phase transition in a Hubbard model on a quasionedimentional twoleg ladder.
The existence of a quantum phase transition in a Hubbard model on a quasionedimentional twoleg ladder. Valentin Voroshilov Physics Department, Boston University, Boston, MA, 02215, USA A canonical transformation
More informationAtoms, Molecules and Solids (selected topics)
Atoms, Molecules and Solids (selected topics) Part I: Electronic configurations and transitions Transitions between atomic states (Hydrogen atom) Transition probabilities are different depending on the
More informationChapter 23. Transition Metals and Coordination Chemistry
Chapter 23 Transition Metals and Coordination Chemistry The Transition Metals: Exact Definition Transition metal: An element whose atom has an incomplete d subshell or which can give rise to cations with
More informationScanning tunneling microscopy of monoatomic gold chains on vicinal Si(335) surface: experimental and theoretical study
phys. stat. sol. (b) 4, No., 33 336 (005) / DOI 10.100/pssb.00460056 Scanning tunneling microscopy of monoatomic gold chains on vicinal Si(335) surface: experimental and theoretical study M. Krawiec *,
More informationMesoscopic NanoElectroMechanics of Shuttle Systems
* Mesoscopic NanoElectroMechanics of Shuttle Systems Robert Shekhter University of Gothenburg, Sweden Lecture1: Mechanically assisted singleelectronics Lecture2: Quantum coherent nanoelectromechanics
More informationQuantum Monte Carlo Simulations of the Halffilled Hubbard Model. Anders F. J. Gabrielsson
Quantum Monte Carlo Simulations of the Halffilled Hubbard Model Anders F. J. Gabrielsson June 2011 Abstract A Quantum Monte Carlo method of calculating operator expectation values for the ground state
More informationPhenomenology and Models of Exchange Bias in Core /Shell Nanoparticles
Phenomenology and Models of Exchange Bias in Core /Shell Nanoparticles Xavier Batlle and Amílcar Labarta Departament de Física Fonamental and Institut de Nanociència i Nanotecnologia Universitat de Barcelona,
More informationarxiv: v2 [condmat.strel] 1 Jun 2007
Electronic reconstruction at SrMnO 3 LaMnO 3 superlattice interfaces Şerban Smadici, 1 Peter Abbamonte, 1 Anand Bhattacharya, Xiaofang Zhai, 1 Andrivo Rusydi, 3 James N. Eckstein, 1 Samuel D. Bader, and
More informationMatSci 224 Magnetism and Magnetic. November 5, 2003
MatSci 224 Magnetism and Magnetic Materials November 5, 2003 How small is small? What determines whether a magnetic structure is made of up a single domain or many domains? d Single domain d~l d d >> l
More informationSurfaces, Interfaces, and Layered Devices
Surfaces, Interfaces, and Layered Devices Building blocks for nanodevices! W. Pauli: God made solids, but surfaces were the work of Devil. Surfaces and Interfaces 1 Role of surface effects in mesoscopic
More informationElectron spins in nonmagnetic semiconductors
Electron spins in nonmagnetic semiconductors Yuichiro K. Kato Institute of Engineering Innovation, The University of Tokyo Physics of noninteracting spins Optical spin injection and detection Spin manipulation
More informationFrom Last Time Important new Quantum Mechanical Concepts. Atoms and Molecules. Today. Symmetry. Simple molecules.
Today From Last Time Important new Quantum Mechanical Concepts Indistinguishability: Symmetries of the wavefunction: Symmetric and Antisymmetric Pauli exclusion principle: only one fermion per state Spin
More informationIntermission: Let s review the essentials of the Helium Atom
PHYS3022 Applied Quantum Mechanics Problem Set 4 Due Date: 6 March 2018 (Tuesday) T+2 = 8 March 2018 All problem sets should be handed in not later than 5pm on the due date. Drop your assignments in the
More informationMagnetic domain theory in dynamics
Chapter 3 Magnetic domain theory in dynamics Microscale magnetization reversal dynamics is one of the hot issues, because of a great demand for fast response and high density data storage devices, for
More informationMagnetic Force on a Moving Charge
Magnetic Force on a Moving Charge Electric charges moving in a magnetic field experience a force due to the magnetic field. Given a charge Q moving with velocity u in a magnetic flux density B, the vector
More informationTopological insulator with timereversal symmetry
Phys620.nb 101 7 Topological insulator with timereversal symmetry Q: Can we get a topological insulator that preserves the timereversal symmetry? A: Yes, with the help of the spin degree of freedom.
More informationWangLandau sampling for Quantum Monte Carlo. Stefan Wessel Institut für Theoretische Physik III Universität Stuttgart
WangLandau sampling for Quantum Monte Carlo Stefan Wessel Institut für Theoretische Physik III Universität Stuttgart Overview Classical Monte Carlo First order phase transitions Classical WangLandau
More informationPRINCIPLES OF ADSORPTION AND REACTION ON SOLID SURFACES
PRINCIPLES OF ADSORPTION AND REACTION ON SOLID SURFACES Richard I. Masel Department of Chemical Engineering University of Illinois at UrbanaChampaign Urbana, Illinois A WILEYINTERSCIENCE PUBLICATION
More informationarxiv:condmat/ v1 4 Oct 2002
Current induced spin wave excitations in a single ferromagnetic layer Y. Ji and C. L. Chien Department of Physics and Astronomy, The Johns Hopkins University, Baltimore, Maryland arxiv:condmat/0210116v1
More information5 Topological insulator with timereversal symmetry
Phys62.nb 63 5 Topological insulator with timereversal symmetry It is impossible to have quantum Hall effect without breaking the timereversal symmetry. xy xy. If we want xy to be invariant under, xy
More informationPhase Transitions in Relaxor Ferroelectrics
Phase Transitions in Relaxor Ferroelectrics Matthew Delgado December 13, 2005 Abstract This paper covers the properties of relaxor ferroelectrics and considers the transition from the paraelectric state
More informationTypes of Magnetism and Magnetic Domains
Types of Magnetism and Magnetic Domains Magnets or objects with a Magnetic Moment A magnet is an object or material that attracts certain metals, such as iron, nickel and cobalt. It can also attract or
More informationIntroduction to Nanotechnology Chapter 5 Carbon Nanostructures Lecture 1
Introduction to Nanotechnology Chapter 5 Carbon Nanostructures Lecture 1 ChiiDong Chen Institute of Physics, Academia Sinica chiidong@phys.sinica.edu.tw 02 27896766 Carbon contains 6 electrons: (1s) 2,
More informationMetalinsulator transitions
Metalinsulator transitions What can we learn from electronic structure calculations? Mike Towler mdt26@phy.cam.ac.uk www.tcm.phy.cam.ac.uk/ mdt26 Theory of Condensed Matter Group Cavendish Laboratory
More informationChapter 8: Magnetic and Electrical Properties
Chapter 8: Magnetic and Electrical Properties 1 In solids, properties of individual atoms can interact cooperatively to produce effects not found in fluids. Magnetic Susceptibility: magnetic field produces
More informationEXTRINSIC SEMICONDUCTOR
EXTRINSIC SEMICONDUCTOR In an extrinsic semiconducting material, the charge carriers originate from impurity atoms added to the original material is called impurity [or] extrinsic semiconductor. This Semiconductor
More informationChris G. Van de Walle
Complex oxide interfaces Chris G. Van de Walle Anderson Janotti, Lars Bjaalie, Luke Gordon, Burak Himmetoglu, K. Krishnaswamy Materials Department, University of California, Santa Barbara ES213 June 1114,
More informationInteracting Fermi Gases
Interacting Fermi Gases Mike Hermele (Dated: February 11, 010) Notes on Interacting Fermi Gas for Physics 7450, Spring 010 I. FERMI GAS WITH DELTAFUNCTION INTERACTION Since it is easier to illustrate
More informationExtraordinary Hall effect in FeCr giant magnetoresistive multilayers
PHYSICAL REVIEW B 68, 144405 2003 Extraordinary Hall effect in FeCr giant magnetoresistive multilayers P. Khatua and A. K. Majumdar* Department of Physics, Indian Institute of Technology, Kanpur  208016,
More informationRole of Hund Coupling in TwoOrbital Systems
Role of Hund Coupling in TwoOrbital Systems Gun Sang Jeon Ewha Womans University 20130830 NCTS Workshop on Quantum Condensation (QC13) collaboration with A. J. Kim, M.Y. Choi (SNU) MottHubbard Transition
More informationBasics of DFT applications to solids and surfaces
Basics of DFT applications to solids and surfaces Peter Kratzer Physics Department, University DuisburgEssen, Duisburg, Germany Email: Peter.Kratzer@uniduisburgessen.de Periodicity in real space and
More informationMagnetic Field Lines for a Loop
Magnetic Field Lines for a Loop Figure (a) shows the magnetic field lines surrounding a current loop Figure (b) shows the field lines in the iron filings Figure (c) compares the field lines to that of
More information